Solvent modulation in peptide sub-micro ﬁ bers obtained by solution blow spinning
Ana Margarida Gonçalves Carvalho Dias1,2
*, Cícero Cena3
, Viviane Lutz-Bueno4,5
, Raffaele Mezzenga4
, Ana Marques6,7
, Isabel Ferreira6
and Ana Cecília Afonso Roque1,2
1Associate Laboratory i4HB, Chemistry Department, NOVA School of Science and Technology, Institute for Health and Bioeconomy, Caparica, Portugal,2UCIBIO—Applied Molecular Biosciences Unit, Department of Chemistry, NOVA School of Science and Technology, NOVA University Lisbon, Caparica, Portugal,3UFMS—Federal University of Mato Grosso do Sul, Campo Grande, Brazil,
4Department of Health Sciences and Technology, ETH Zürich, Zürich, Switzerland,5Paul Scherrer Institute, Villigen PSI, Switzerland,6i3N, Materials Department, School of Science and Technology, NOVA University Lisbon, Caparica, Portugal,7Physics Department, Faculty of Sciences, University of Lisbon, Lisbon, Portugal
Peptides possess high chemical diversity at the amino acid sequence level, which further translates into versatile functions. Peptides with self-assembling properties can be processed into diverse formats giving rise to bio-based materials. Peptide-based spun ﬁbers are an interesting format due to high surface-area and versatility, though theﬁeld is still in its infancy due to the challenges in applying the synthetic polymer spinning processes to protein ﬁbers to peptides. In this work we show the use of solution blow-spinning to produce peptideﬁbers. Peptideﬁber formation was assisted by the polymer poly (vinyl pyrrolidone) (PVP) in two solvent conditions. Peptide miscibility and further self-assembling propensity in the solvents played a major role inﬁber formation. When employing acetic acid as solvent, peptideﬁbers (0.5μm) are formed around PVPﬁbers (0.75μm), whereas in isopropanol only one type of ﬁbers are formed, consisting of mixed peptide and PVP (1μm). This report highlights solvent modulation as a mean to obtain different peptide sub- microﬁbers via a single injection nozzle in solution blow spinning. We anticipate this strategy to be applied to other small peptides with self- assembly propensity to obtain multi-functional proteinaceousﬁbers.
peptide-basedﬁbers, solution blow-spinning, polymericﬁbers, solvent modulation, self-assembly
Nature is a source of inspiration to produce innovative, sustainable and biodegradable materials (Katiyar et al., 2021). Peptides with self-assembling properties are interesting molecules to form bio-based materials, as they are composed by a small sequence of amino acids that can be derived from natural sequences, rationally designed or discovered through screening protocols (Berger and
OPEN ACCESS EDITED BY Francesca D’Anna, University of Palermo, Italy
REVIEWED BY Kai Tao,
Zhejiang University, China Antonietta Pepe,
University of Basilicata, Italy
Ana Margarida Gonçalves Carvalho Dias, firstname.lastname@example.org
Ana Cecília Afonso Roque, email@example.com
This article was submitted to Supramolecular Chemistry, a section of the journal Frontiers in Chemistry
RECEIVED26 September 2022 ACCEPTED21 November 2022 PUBLISHED06 December 2022
Dias AMGC, Cena C, Lutz-Bueno V, Mezzenga R, Marques A, Ferreira I and Roque ACA (2022), Solvent modulation in peptide sub-microﬁbers obtained by solution blow spinning.
© 2022 Dias, Cena, Lutz-Bueno, Mezzenga, Marques, Ferreira and Roque. This is an open-access article distributed under the terms of the Creative Commons Attribution License (CC BY). The use, distribution or reproduction in other forums is permitted, provided the original author(s) and the copyright owner(s) are credited and that the original publication in this journal is cited, in accordance with accepted academic practice. No use, distribution or reproduction is permitted which does not comply with these terms.
TYPEOriginal Research PUBLISHED06 December 2022 DOI10.3389/fchem.2022.1054347
Gazit, 2017). Compared to long protein sequences with self- assembly propensity, peptides composed by natural and non- natural amino acids have advantages: they are easy and inexpensive to produce through chemical synthesis in a reliable and scalable manner; they are soluble in water or in non-toxic solvents (Dias et al., 2015;Dias et al., 2016); and they are easily assessed by biophysical and structural studies (Sánchez-Ferrer et al., 2018; Lutz-Bueno et al., 2020).
Recently, theﬁeld of peptide-based materials has seen great advances due to an increasing understanding of peptide self- assembling principles into higher-ordered structures at the nano-, micro- and even macro-scales (Shaham-Niv et al., 2015;Balasco et al., 2021).
Self-assembled peptides have been traditionally explored to produce hydrogels with various applications in biomedicine and sensing (Amit et al., 2018;Balasco et al., 2021). Recently, it has been acknowledged the untapped opportunities of peptide- basedﬁbers, namely the large surface to aspect ratio associated with large chemical diversity, facile sequence design allow access to different nanoscale architectures, and tunability of optical and electrical properties (Yıldız et al., 2020;Bucci et al., 2021a; Kim et al., 2021). It is known that proteins or small protein precursors (e.g. soya, elastin, spider silk protein or hemoglobin) can be processed by electrospinning to generate protein-ﬁbers for biomaterials and bio-based materials (DeFrates et al., 2018; Yıldız et al., 2020). It has also been demonstrated that peptide sequences composed by hydrophobic amino acids (e.g. Tyrosine, Phenylalanine, Tryptophan), which can naturally self-assemble due to hydrophobic interactions (e.g. π-π stacking), can also form ﬁbers (Balasco et al., 2021). A recent review compiled successful examples of peptide sequences that were spun into ﬁbers through electrospinning (Bucci et al., 2021a). Despite
these successes, the main identiﬁed challenges to obtain peptide ﬁbers are the low viscosity of peptide solutions, thus requiring high amounts of peptide (10–50% wt/v) to be spun or combination with a polymer (Kim et al., 2021), and the toxicity of solvents used (e.g. hexaﬂuoro-2-propanol (HFIP) and triﬂuoroacetic acid (TFA)) with a pressing need for more sustainable solutions (Bucci et al., 2021a). Solution blow spinning (SBS) is an alternative method to electrospinning, with advocated main advantages of high production rate and easy implementation (Dadol et al., 2020;Gao et al., 2021). SBS has been used to yield materials from a wide range of natural and synthetic polymers or blends, such as Soya Protein, cellulose, chitosan, poly (vinylidene ﬂuoride), poly (vinyl pyrrolidone) (PVP), poly (L-lactic acid) or poly (vinyl acetate) (Dos Santos et al., 2020). PVP is a low-cost synthetic polymer with low toxicity and good solubility in water or polar solvents. Due its high solubility, PVP can be removed after ﬁbers production by placing them in water (Kurakula and Rao, 2020). Polymer ﬁbers are normally coated with peptides as a post-treatment by physical adsorption or by chemical means (Dart et al., 2019; Butruk- Raszeja et al., 2020;Bucci et al., 2021b;Yao et al., 2023).
In this work, we aim to advance the knowledge on peptide- ﬁber formation using SBS. We explore a peptide-polymer blend to obtain the desired viscosity at lower peptide concentrations, and by selecting greener solvents (acetic acid and isopropanol (Byrne et al., 2016)) for operation. We used as a proof-of-concept a peptide sequence that self-assembles into higher-ordered structures, identiﬁed as the protopeptide YMDMSGYQ, that derives from structural proteins (reﬂectins) present in cephalopods (Guan et al., 2017). It is postulated that the Tyrosine amino acids in the peptide sequence lead to the self- assembly of the peptide byπ-πstacking interactions (Guan et al.,
2017). We observed that by changing the solvent we could achieve ﬁbers with different morphologies and diameters.
Consequently, we concluded that we can obtain ﬁbrous materials with different properties by solvent modulation.
2 Materials and methods
The peptide YMDMSGYQ was chemically synthesized (Triﬂuoroacetic acid free and free terminals) with 97% purity at Genecust (France). Poly (vinyl pyrrolidone) Molecular Weight 360000Da powder, Congo red BioXtra grade, sodium chloride, acetic acid glacial>99% and isopropanol>99% were purchased from Sigma-Aldrich.
2.2 Fiber production by solution blow- spinning
Four different solutions (1.6–2.0 ml) were prepared (Supplementary Table S1): PVP AA was composed by PVP in 80:20 (v/v) acetic acid in water; PVP Pep AA was composed by PVP and peptide in 80:20 (v/v) acetic acid in water; PVP Iso was composed by PVP in 70:30 (v/v) isopropanol in water;
PVP Pep Iso consisted of PVP and peptide in 70:30 (v/v) isopropanol in water. The solutions were prepared by dissolving PVP (10% wt/v) in the solvent at 40°C under magnetic stirring, after which 100μl of a peptide solution (Pep AA or Pep Iso at 12% wt/v) in each solvent. Theﬁnal mixture was composed by PVP (10% wt/v) and peptide (0.75%
wt/v). The mixture was incubated for 10 min at 40°C with continuous agitation. A syringe cleaned with the solvent was loaded with the solution and ﬁbers were prepared using a solution blow spinning setup as described elsewhere (Cena et al., 2018). Theﬂow rate used was 0.05 ml/min with an air pressure of 1 MPa. Fibers were projected into a static target with a 50 cm working distance from the nozzle. The ﬁber spinning was conducted in a room with temperature of 21°C and with relative humidity of 60–70%.
2.3 Congo red staining
Solution orﬁbers produced by SBS (50μl) were placed in a glass slide, and 20μl of Congo red solution (20 mg in 10 ml of saturated ethanol solution (2.5 g NaCl with 80% EtOH) (Yakupova et al., 2019)) were added. Any excess of Congo red solution was removed with a lint free paper. The glass slides were observed at the ZEISS Axio Observer Microscope 5, 10, and 40 objectives and under brightﬁeld and cross-polarized ﬁlters (90°angle).
2.4 Atomic force microscopy
All polymer and polymer-peptide solutions (10μl) were loaded into mica layer and dried overnight in a dust free environment. The surface topography and roughness of viscous solutions were analyzed with the Atomic Force Microscope integrated in the WITec Alpha 300 RAS confocal spectrometer. The cantilever was operated with an Al coated probe in AC mode at 75 kHz and constant load of 2.8 N/m.
Lateral and depth resolutions were 1 nm and 0.3 nm, respectively.
For all sample’s roughness was determined through the topography maps root mean square height (Sq).
2.5 Scanning electron microscopy (SEM)
Scanning electron microscopy (SEM) observations were conducted on a Carl Zeiss AURIGA CrossBeam (FIB-SEM) workstation coupled with energy dispersive X-ray spectroscopy (EDS, Oxford X-Max 150 detector with Aztec software). It was also used TM3030Plus tabletop Microscope from Hitachi. The ﬁbers were previously coated with an Pd conductiveﬁlm to avoid charge effects.
2.6 Attenuated total re ﬂ ectance – Fourier transform infrared spectroscopy
Fourier-transform infrared spectroscopy (ATR-FTIR) characterization of theﬁbers. PVPﬁbers and PVP-Peptideﬁbers produced in solvents and deuterium water. Spectra were recorded using Spectrum Two with UTAR two adapter from Perkin Elmer.
Scans were recorded in absorption mode and as a background air was used. It was used force gauge of 83. In total 25 scans were obtained and averaged with the range from 4000 to 400cm−1.
2.7 Small-angle X-ray scattering (SAXS) and wide-angle X-ray scattering (WAXS)
The scattering measurements were performed with Rigaku MicroMax-002+ micro-focused beam (4 kW, 45 kV, and 0.88 mA). The copper Kα energy with λe = 1.54 Å was collimated by three pinholes onto a beam size of 700 × 700μm2. A two-dimensional argon-ﬁlled Triton detector was used for collecting SAXS patterns, and a Fuji Film BAS-MS 2025 imaging plate for WAXS. The active range q = 0.001–0.200 Å−1was probed for SAXS, and q = 0.2–2.5 Å−1for WAXS. Polymer only and polymer-peptideﬁbers (PVP AA, PVP Pep AA, PVP Iso and PVP Pep Iso) with diameters between 0.1 and 3 µm were vertically mounted, and measured simultaneously by WAXS and SAXS for 3 h (Lara et al., 2012;
Lutz-Bueno et al., 2020).
Dias et al. 10.3389/fchem.2022.1054347
3 Results and discussion
Peptide solutions can be processed intoﬁbers using spinning procedures (Khadka and Haynie, 2012;Dart et al., 2019;Hosseini et al., 2019; Yıldız et al., 2020; Kim et al., 2021). Still, improvements are needed to accommodate the low viscosity of peptide solutions and the low sustainability of solvents used during spinning (Bucci et al., 2021a). We approached these challenges by adding a polymer to the peptide solution to promote ﬁber formation at lower peptide concentrations (0.75% wt/v). In addition, we attempted the dissolution of the peptide and polymer in environmentally friendly solvents, namely acetic acid and isopropanol, and testedﬁber formation by solution blow spinning (SBS).
The peptide sequence YMDMSGYQ was selected as a model peptide for our studies. This octapeptide has two Tyrosine residues in the extremities of the sequence, which are suggested to promote peptide self-assembly and further organization into higher- ordered structures (Guan et al., 2017). Tyrosine residues promote π-π stacking and hydrogen bond interactions due to the tyrosyl side chain, allowing for mixed mode intermolecular
interactions (Lee et al., 2019). In fact, we conducted preliminary studies which show that the peptide self-assembly is concentration and time-dependent in aqueous media at low pH, giving rise to hydrogels. The peptide self-assembles into nanoﬁbers as determined by AFM (Supplementary Figure S1A). The adopted secondary structure is likely strongly inﬂuenced by stacking of aromatic residues, showing an intense peak at 230 nm in Circular Dichroism (Supplementary Figure S1B), and it is predominantly based onβ-sheets, due to an intense peak at 1615 cm−1observed by deconvolution of Attenuated total reﬂectance–Fourier transform infrared spectroscopy (ATR-FTIR) spectrum in Amide I region (1700 and 1600 cm−1) (Supplementary Figure S1C).
To increase the viscosity of peptide solutions, we combined the peptide with PVP. PVP is the most used synthetic polymer to produceﬁbers by solution blow spinning (Dadol et al., 2020;Dos Santos et al., 2020) and it has high solubility in water and polar solvents (Kurakula and Rao, 2020) (Figure 1A). We selected two solvents to dissolve PVP and the peptide: 1) 80:20 (v/v) acetic acid in water, and 2) 70:30 (v/v) isopropanol in water (Figure 1B).
These solvents were selected as both are less toxic than the traditional hexaﬂuoro-2-propanol (HFIP) and triﬂuoroacetic
(A)Structures of the components used in this work: Polymer—PVP and peptide—Protopeptide;(B)Research strategy to produceﬁbers using solutions with polymer and peptide in two different solvents: 80% acetic acid (80:20 (v/v) acetic acid in water) and 70% Isopropanol (70:30 (v/v) isopropanol in water). The method to spun the solutions into theﬁbers was solution blow spinning.(C)Macroscopicﬁbers obtained through solution blow spinning.
acid (TFA) and present high volatility. Four aqueous solutions were then prepared as starting materials for SBS processing: PVP only (PVP AA), PVP with Peptide (PVP Pep AA) in 80:20 (v/v) acetic acid in water; and PVP only (PVP Iso) and PVP with peptide (PVP Pep Iso) in 70:30 (v/v) isopropanol in water (Supplementary Table S1).
Acetic acid is a polar solvent that mostly contributes as an H-bond acceptor. Isopropanol can establish hydrophobic interactions through the alkyl chain and hydrogen bonds through the H-bond donor capabilities of the alcohol group. PVP has a carbonyl group that is a H-bond acceptor, and it also presents a negative charge at most pH values (isoelectric point (pI) < 3). PVP can form different interactions in acetic acid and isopropanol and it is in fact known to be highly soluble in water, isopropanol and acetic acid (Cena et al., 2018). We observed a proper solubilization of PVP in both solvents (Supplementary Figure S2A). The peptide presents a low pI (pI = 3.7) being positively charged in acetic acid solution (peptide solution with pH 2–3), and neutral to slightly negative in the isopropanol solution (peptide solution with pH 4). Being an octapeptide, it can establish a multitude of interactions, namely hydrophobic and hydrogen bonds through the backbone (both as H-bond donor and acceptor) and through amino acids side chains, such as Tyrosine, Glutamine, Serine and Aspartic acid residues. The peptide was readily dissolved in the acetic acid solution yielding a transparent solution (Pep AA, Supplementary Figure S2A). By adding the peptide to the PVP solution in acetic acid (PVP Pep AA) the transparency of the solution was maintained, but it was possible to observe the formation of peptide aggregates upon Congo red staining, which were less visible in the solution containing only peptide (control) (Supplementary Figure S2B). This indicates that the peptide can self-assemble into ordered structures in the acetic acid solution with PVP polymer. Conversely, the dissolution of peptide in isopropanol resulted in a whiteﬂocculated solution with poor solubility, yielding large peptide aggregates with green birefringence when stained with Congo red (Pep Iso, Supplementary Figures S2A,B). However, when the peptide solution was added to the PVP solution in isopropanol (PVP Pep Iso) and incubated at 40°C, a translucid solution was formed suggesting an improvement in peptide solubility in the presence of the polymer. This result was conﬁrmed by the absence of peptide aggregates when staining with Congo Red (Supplementary Figure S2B). In PVP Pep Iso solution we may have predominantly hydrophobic interactions between the peptide (which is neutral to weekly negative) and the polymer chain, which are favored by the presence of isopropanol.
The solutions were further characterized by AFM (Supplementary Figure S3), and it was visible the presence of aggregates in PVP Pep AA, in contrast with PVP Pep Iso, which presents a surface with some texture. Besides, to quantify the roughness in the mica surface it was determined the root mean square height (Sq) for all samples (Supplementary Figure S3C).
PVP Pep AA displays the highest Sq among all samples, thus indicating large volumes in the surface of the mica. These large volumes can indicate that there are aggregates of peptide. In solutions of PVP Pep Iso, the opposite occurs with lowest values of roughness. These results agree with the observations of Congo red staining. Thus, in presence of the polymer, the peptide self- assembles into higher-order aggregates in acetic acid and it is in a monomeric format in isopropanol.
The solutions were then processed into ﬁbers by solution blow spinning and all yielded ﬁbers (Figure 2). The control solution PVP AA gave rise to ﬁbers with several morphological defects as “dried particles” and beads, whereas PVP Iso originated well-deﬁnedﬁbers (smooth and cylindrical) (Figure 2A; Supplementary Figure S4A). PVP Pep AA also presented well-deﬁned ﬁbers with different diameters and PVP Pep Iso demonstrate a mixture of ﬁbers with morphological defects as “beads” and “dried particles” (Cena et al., 2018). The diameter of the differentﬁbers was measured (except for the PVP AA control due to the high number of defects) and a monomodal ﬁber diameter distribution was observed (Figure 2B). The PVP Iso ﬁbers showed a wide diameter distribution from 0.50–2.75 µm, centered around 1.34 µm. A narrow ﬁber diameter distribution was observed for PVP Pep AA, with the diameter centered around 0.68 µm.
The PVP Pep Isoﬁbers showed an intermediaryﬁber diameter distribution, centered around 0.96 µm, between PVP Iso and PVP Pep AA. Adding the peptide to the PVP solution induces the formation of thinnerﬁbers, probably by reducing the viscosity of the solutions, as veriﬁed before (Farias et al., 2020). Despite some variability, allﬁbers diameters are well in accordance with the data described in the literature for solution blow-spinning (Cena et al., 2018).
A further question arose on how the peptide assembled in the ﬁbers (Figure 2C;Supplementary Figures S4, S5). In the case of PVP Pep AA ﬁbers, we observed the presence of distinct ﬁbers upon Congo red staining–a main ﬁber and a secondaryﬁber, which is a thinner entangledﬁber. In bright ﬁeld both ﬁbers stained red, however under cross polarized light only the thinnerﬁber presented green birefringence. This is typically associated with peptide and protein-based amyloid or amyloid-like aggregates (Shaham-Niv et al., 2015;
Yakupova et al., 2019), suggesting that the thinner ﬁber contains higher amounts of organized peptide structures and the main ﬁber contains mainly the PVP polymer. In contrast, for PVP Pep Iso only one ﬁber is visible, and it also presents areas with green birefringence upon Congo red staining, indicating that the peptide is co-organized into higher order structures in the presence of PVP polymer.
Theﬁbers were also characterized by ATR-FTIR. When we compared the spectra ofﬁbers with PVP and peptide, we do not see major differences from the control with PVP only. This is due to the low amount of peptide in the mixture, with PVP spectra masking peptide peaks. Control PVP ﬁbers present
Dias et al. 10.3389/fchem.2022.1054347
intense characteristic peaks C=O at 1660cm−1 and C-N stretching at 1264cm−1 (Cena et al., 2018) (Supplementary Figure S6). The deconvolution of Amide I band was not possible, and we could not use this method to infer on the secondary structure of the peptide within theﬁbers.
Fibers were also characterized by X-ray scattering in an attempt to understand the assembly of the peptide within the ﬁbers.Figure 2Dcompares the WAXS signal as integrated curves from the differentﬁbers, after normalizing their intensity by the maximum intensity value. For all ﬁbers independent of the
Characterization of polymer and peptideﬁbers produced by Solution Blow Spinning.(A)SEM analysis ofﬁbers produced in 80% Acetic Acid (AA) and 70% isopropanol (Iso). It was observed several defects in PVP AAﬁbers and all the other samples presentﬁbers without defects.(B)Histogram of theﬁbers diameter for samples: PVP Pep AA, PVP Pep Iso and PVP Iso.(C)In the upper panel, microscopic observation of Congo red staining for PVP Pep AA and PVP Pep Isoﬁbers. In PVP Pep AA, in brightﬁeld are observed twoﬁbers: one mainﬁber in red and a second thinnerﬁber, but under polarizedﬁeld (cross polarized at 90°angle) only the thinnerﬁber presents green birefringence. In PVP Pep Iso, only oneﬁber is observed in bright ﬁeld and in polarizedﬁeld has areas with green birefringence. In the lower panel, schematic of the microscopic observations, for the PVP with peptide ﬁbers obtained in the different solvents: a mainﬁber of PVP (black), a peptideﬁber (green) and aﬁber that contain both compounds (grey).(D)WAXS, the P1 and P2 identify two main peaks observed in the differentﬁbers.(E)SAXS data for the differentﬁbers, the arrow identiﬁes a weak correlation peak.
solvent, the WAXS signal has two reﬂection peaks–P1 ~ 0.8 Å-1 and P2 ~ 1.35–1.39 Å-1. We assign these peaks to the reﬂections at 0.7 and 1.2 Å-1, which are characteristicﬁngerprints of polymers (Busselez et al., 2012). These results suggest that the peptide signals of a possible amyloid structure, beta-sheets or beta- strands are being masked by the strong PVP signals that occur in the same q-range. Due to the overlap of signals, it is not possible to identify the structure of the peptides within these ﬁbers. However, the main difference between these samples is that PVP Pep ﬁbers exhibit higher intensities for P2 in both solvents. This peak is usually associated with hydrogen bond interactions in amyloids, and it is related to beta-strands. Thus, these results suggest the presence of a compound in theﬁber that promotes these interactions. In fact, from previous studies to determine the secondary structure of the peptide by circular dichroism, we identiﬁed a strong beta-sheet secondary structure content when the peptide assembles into higher structures (Supplementary Figure S1). The SAXS curves indicated a weak correlation peak at q ~ 1 A−1(Figure 2E, arrow), which indicates that theseﬁbers have a certain regularity in spacing in the length
scale of about 63 Å. From complementary studies with this peptide, we speculate that such dimension of 63 Å could be related to the distance between the peptide’s chains (data not shown).
It should be noted that the formation of peptide-onlyﬁbers has been attempted. Peptide solutions in 80:20 (v/v) acetic acid in water were prepared at concentrations 0.75, 3, 5, 7.5, and 15% wt/v and the viscosity measured in a rotary viscosimeter. It was observed a linear correlation between the concentration and viscosity of the solutions until 5%wt/v. For higher concentrations, the viscosity measurements were very unsatisfactory, since as soon as the solution was deposited in a surface, the solvent would evaporate, and the peptide gelate (Table 1). Despite that, the 15% wt/v solution showed the highest viscosity results and closer to the desired viscosity for SBS (0.45–0.5 Pa.S) (Cena et al., 2018). However, when attempting to process the 15% wt/v solution by SBS, the peptide started to gelate as soon as the solvent evaporate in the tip of the nozzle, due to the high concentration. Thus, the peptide in acetic acid self-assembles at concentrations ideal for SBS, but it is difﬁcult to have the perfect balance between peptide concentration, viscosity and gelation control.
Therefore, the use of PVP to co-spin peptide ﬁbers contributes for an ideal viscosity of the peptide solutions. In addition, PVP can be removed afterﬁbers production due to its water solubility. We veriﬁed this second advantage by placing PVP Pep AA and PVP Pep Isoﬁbers in a glass slide which was wet with water to solubilize PVP. In Figure 3it is possible to observe oneﬁber with some fragments suggesting that PVP was dissolved, especially visible in the PVP Pep AA sample. Thisﬁber was further stained with Congo red and it presented green birefringence (suggesting the presence of organized peptide assemblies) whereas the small fragments did not.
TABLE 1 Viscosity measurement of peptide solutions in 80:20 (v/v) acetic acid in water using CAP 2000+Viscosimeter (AMETEK Brookﬁeld) following manufacturer instructions.
Peptide concentration (% wt/v) Viscosity (Pa.S)
0.75 0.15 ± 0.01
3 0.20 ± 0.02
5 0.29 ± 0.02
7.5 0.19 ± 0.04
15 0.34 ± 0.04
Microscopic observation of PVP and peptideﬁbers dissolution and staining with Congo Red in bright and polarizedﬁeld (cross polarized at 90° angle).
Dias et al. 10.3389/fchem.2022.1054347
We describe a strategy for solvent modulation to obtain different peptide ﬁbers with only one injection nozzle using solution blow spinning. Our results demonstrate that the miscibility of the peptide in different solvents in the presence of PVP induces the production of ﬁbers with distinct morphologies. In particular, the propensity for peptide self- assembly in distinct solvents seems to be the key aspect to induce the formation of PVP-enriched and peptide-enriched ﬁbers (as in the case of acetic acid) or the formation of co- assembled ﬁbers PVP-peptide (in isopropanol). Furthermore, PVP ﬁbers can be dissolved without impairing peptide ﬁber integrity. This solvent modulation strategy opens a new approach for production of peptides-based ﬁbers for different bioengineering applications.
Data availability statement
The raw data supporting the conclusion of this article will be made available by the authors, without undue reservation.
AD and CC designed the experiments and wrote the manuscript. AD conducted the experiments and produced the ﬁrst draft of the manuscript. VL-B and RM contributed with experiments in SAXS and WAXS and wrote the manuscript. AM and IF acquired and prepared the images in AFM and wrote the manuscript. AR contributed for design and conceptualization, revised the manuscript and funding acquisition. All authors listed have made a substantial, crucial and direct contribution to the work, and approved it for publication.
This work has received funding from the European Research Council (ERC) for the project SCENT-ERC-2014-STG-639123 (2015–2022), from CNPq (408127/2018-0) and Fundect (71.700.173/2018)-Brazil, and from Fundação para a Ciência e Tecnologia (Portugal) for projects PTDC/BII-BIO/28878/2017, PTDC/CTM-CTM/3389/2021, UIDP/04378/2020, and UIDB/
04378/2020 of the Research Unit on Applied Molecular Biosciences–UCIBIO, and the project LA/P/0140/2020 of the Associate Laboratory Institute for Health and Bioeconomy—i4HB, as well as Iana Lycko PhD grant (SFRH/BD/147388/2019).
Con ﬂ ict of interest
The authors declare that the research was conducted in the absence of any commercial orﬁnancial relationships that could be construed as a potential conﬂict of interest.
Publisher ’ s note
All claims expressed in this article are solely those of the authors and do not necessarily represent those of their afﬁliated organizations, or those of the publisher, the editors and the reviewers. Any product that may be evaluated in this article, or claim that may be made by its manufacturer, is not guaranteed or endorsed by the publisher.
The Supplementary Material for this article can be found online at: https://www.frontiersin.org/articles/10.3389/fchem.
Amit, M., Yuran, S., Gazit, E., Reches, M., and Ashkenasy, N. (2018). Tailor-made functional peptide self-assembling nanostructures.Adv. Mat.30 (41), 1707083.
Balasco, N., Diaferia, C., Morelli, G., Vitagliano, L., and Accardo, A. (2021).
Amyloid-like aggregation in diseases and biomaterials: Osmosis of structural information.Front. Bioeng. Biotechnol.9, 641372. doi:10.3389/fbioe.2021.641372 Berger, O., and Gazit, E. (2017). Molecular self-assembly using peptide nucleic acids.Biopolymers108 (1), 229300–e23010. doi:10.1002/bip.22930
Bucci, R., Georgilis, E., Bittner, A. M., Gelmi, M. L., and Clerici, F. (2021).
Peptide-based electrospun ﬁbers: Current status and emerging developments.
Nanomater. MDPI Ag.11 (5), 1–22. doi:10.3390/nano11051262
Bucci, R., Vaghi, F., Erba, E., Romanelli, A., Gelmi, M. L., and Clerici, F. (2021).
Peptide grafting strategies before and after electrospinning of nanoﬁbers.Acta Biomater.122, 82–100. doi:10.1016/j.actbio.2020.11.051
Busselez, R., Arbe, A., Cerveny, S., Capponi, S., Colmenero, J., and Frick, B.
(2012). Component dynamics in polyvinylpyrrolidone concentrated aqueous solutions.J. Chem. Phys.137 (8), 084902. doi:10.1063/1.4746020
Butruk-Raszeja, B. A., Kuzminska, A., Wojasinski, M., and Piotrowska, Z. (2020).
Physicochemical and mechanical properties of blow spun nanoﬁbrous prostheses modiﬁed with acrylic acid and REDV peptide.Coatings10 (1110), 1110–1120.
Byrne, F. P., Jin, S., Paggiola, G., Petchey, T. H. M., Clark, J. H., Farmer, T. J., et al.
(2016). Tools and techniques for solvent selection: Green solvent selection guides.
Sustain. Chem. Process.4 (1), 7–24. doi:10.1186/s40508-016-0051-z
Cena, C. R., Silva, M. J., Malmonge, L. F., and Malmonge, J. A. (2018). Poly(vinyl pyrrolidone) sub-microﬁbers produced by solution blow spinning.J. Polym. Res.25 (11), 238–8. doi:10.1007/s10965-018-1633-0
Dadol, G. C., Kilic, A., Tijing, L. D., Lim, K. J. A., Cabatingan, L. K., Tan, N. P. B., et al. (2020). Solution blow spinning (SBS) and SBS-spun nanoﬁbers: Materials, methods, and applications.Mater Today Commun. [Internet]25, 101656. doi:10.
Dart, A., Bhave, M., and Kingshott, P. (2019). Antimicrobial peptide-based electrospun ﬁbers for wound healing applications. Macromol. Biosci. 19 (9), 1800488–1800516. doi:10.1002/mabi.201800488
DeFrates, K. G., Moore, R., Borgesi, J., Lin, G., Mulderig, T., Beachley, V., et al.
(2018). Protein-basedﬁber materials in medicine: A review.Nanomaterials8 (7), 457. doi:10.3390/nano8070457
Dias, A., dos Santos, R., Iranzo, O., and Roque, A. (2016). Afﬁnity adsorbents for proline-rich peptide sequences: A new role for WW domains. RSC Adv. 6, 68979–68988. doi:10.1039/c6ra10900d
Dias, A., Iranzo, O., and Roque, A. (2015). Anin silicoand chemical approach towards small protein production and application in phosphoproteomics.RSC Adv.
5, 19743–19751. doi:10.1039/c4ra16934d
Dos Santos, D. M., Correa, D. S., Medeiros, E. S., Oliveira, J. E., and Mattoso, L. H.
C. (2020). Advances in functional polymer nanoﬁbers: From spinning fabrication techniques to recent biomedical applications.ACS Appl. Mat. Interfaces12 (41), 45673–45701. doi:10.1021/acsami.0c12410
Farias, R. M. D. C., Mota, M. F., Severo, L. L., Medeiros, E. S. De, Klamczynski, A.
P., Avena-Bustillos, R. D. J., et al. (2020). Green synthesis of porous N-Carbon/Silica nanoﬁbers by solution blow spinning and evaluation of their efﬁciency in dye adsorption.J. Mater. Res. Technol.9 (3), 3038–3046. doi:10.1016/j.jmrt.2020.01.034 Gao, Y., Zhang, J., Su, Y., Wang, H., Wang, X. X., Huang, L. P., et al. (2021).
Recent progress and challenges in solution blow spinning.Mat. Horiz.8 (2), 426–446. doi:10.1039/d0mh01096k
Guan, Z., Cai, T., Liu, Z., Dou, Y., Hu, X., Zhang, P., et al. (2017). Origin of the reﬂectin gene and hierarchical assembly of its protein. Curr. Biol. 27 (18), 2833–2842.e6. doi:10.1016/j.cub.2017.07.061
Hosseini, S. F., Nahvi, Z., and Zandi, M. (2019). Antioxidant peptide-loaded electrospun chitosan/poly(vinyl alcohol) nanoﬁbrous mat intended for food biopackaging purposes.Food Hydrocoll.89 (August2018), 637–648. doi:10.1016/
Katiyar, N. K., Goel, G., Hawi, S., and Goel, S. (2021). Nature-inspired materials:
Emerging trends and prospects.NPG Asia Mat.13 (1), 56. doi:10.1038/s41427-021- 00322-y
Khadka, D. B., and Haynie, D. T. (2012). Protein- and peptide-based electrospun nanoﬁbers in medical biomaterials.Nanomedicine Nanotechnol. Biol. Med.8 (8), 1242–1262. doi:10.1016/j.nano.2012.02.013
Kim, K., Kloxin, C. J., Saven, J. G., and Pochan, D. J. (2021). Nanoﬁbers produced by electrospinning of ultrarigid polymer rods made from designed peptide bundlemers. ACS Appl. Mat. Interfaces 13 (22), 26339–26351. doi:10.1021/
Kurakula, M., and Rao, G. S. N. K. (2020). Pharmaceutical assessment of polyvinylpyrrolidone (PVP): As excipient from conventional to controlled delivery systems with a spotlight on COVID-19 inhibition.J. Drug Deliv. Sci.
Technol.60 (102046), 102046–102124. doi:10.1016/j.jddst.2020.102046 Lara, C., Gourdin-Bertin, S., Adamcik, J., Bolisetty, S., and Mezzenga, R. (2012).
Self-assembly of ovalbumin into amyloid and non-amyloid ﬁbrils.
Biomacromolecules13 (12), 4213–4221. doi:10.1021/bm301481v
Lee, J., Ju, M., Cho, O. H., Kim, Y., and Nam, K. T. (2019). Tyrosine-Rich peptides as a platform for assembly and material synthesis.Adv. Sci.6 (4), 1801255–1801315.
Lutz-Bueno, V., Bolisetty, S., Azzari, P., Handschin, S., and Mezzenga, R. (2020).
Self-winding gelatin–amyloid wires for soft actuators and sensors.Adv. Mat.32 (48), 2004941–2004948. doi:10.1002/adma.202004941
Sánchez-Ferrer, A., Adamcik, J., Handschin, S., Hiew, S. H., Miserez, A., and Mezzenga, R. (2018). Controlling supramolecular chiral nanostructures by self- assembly of a biomimeticβ-sheet-rich amyloidogenic peptide.ACS Nano12 (9), 9152–9161. doi:10.1021/acsnano.8b03582
Shaham-Niv, S., Adler-Abramovich, L., Schnaider, L., and Gazit, E. (2015).
Extension of the generic amyloid hypothesis to nonproteinaceous metabolite assemblies.Sci. Adv.1 (7), e1500137–7. doi:10.1126/sciadv.1500137
Yakupova, E. I., Bobyleva, L. G., Vikhlyantsev, I. M., and Bobylev, A. G. (2019).
Congo Red and amyloids: History and relationship. Biosci. Rep. 39 (1), BSR20181415. doi:10.1042/bsr20181415
Yao, T., Chen, H., Wang, R., Rivero, R., Wang, F., Kessels, L., et al. (2023). Thiol-ene conjugation of a VEGF peptide to electrospun scaffolds for potential applications in angiogenesis.Bioact. Mater.20 (May2022), 306–317. doi:10.1016/j.bioactmat.2022.05.029 Yıldız, A., Kara, A. A., and Acartürk, F. (2020). Peptide-protein based nanoﬁbers in pharmaceutical and biomedical applications. Int. J. Biol. Macromol. 148, 1084–1097. doi:10.1016/j.ijbiomac.2019.12.275
Dias et al. 10.3389/fchem.2022.1054347